Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements


 William Hudson
 1 years ago
 Views:
Transcription
1 Acta Mech. Sin. (2016) 32(2): DOI /s RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1 H. Puga 1 J. Meireles 1 Received: 28 September 2014 / Revised: 15 March 2015 / Accepted: 16 April 2015 / Published online: 17 November 2015 The Chinese Society of Theoretical and Applied Mechanics; Institute of Mechanics, Chinese Academy of Sciences and SpringerVerlag Berlin Heidelberg 2015 Abstract Materials with a negative Poisson s ratio (PR) are called auxetics; they are characterized by expansion/ contraction when tensioned/compressed. Given this counterintuitive behavior, they present very particular characteristics and mechanical behavior. Geometrical models have been developed to justify and artificially reproduce such materials auxetic behavior. The focus of this study is the exploration of a reentrant model by analyzing the variation in the PR of reentrant structures as a function of geometrical and base material parameters. It is shown that, even in the presence of protruding ribs, there may not be auxetic behavior, and this depends on the geometry of each reentrant structure. Values determined for these parameters can be helpful as approximate reference data in the design and fabrication of auxetic lattices using reentrant geometries. Keywords Auxetic Poisson s ratio Reentrant Finite element analysis Elasticity 1 Introduction Poisson s ratio (PR) is a dimensionless constant that describes the negative ratio of lateral strain to the longitudinal strain on a tensioned body. As common sense dictates, the cross section of a body becomes larger/thinner in compression/tension, so the value of this constant is assumed to B V. H. Carneiro 1 Department of Mechanical Engineering, University of Minho, Campus de Azurem, Guimarães, Portugal be positive [1]. However, considering the classical theory of elasticity, it is possible to observe that this constant may assume values from 1 to 0.5 in threedimensional isotropic bodies [2] and between 1 and 1 in twodimensional isotropic materials [3]. For anisotropic materials, this constant depends on the stretch and transverse direction and may assume values other than the previously established ones [4]. Materials that present a generalized negative PR are called auxetics [5]. Anisotropic materials that reveal only negative values of PR along certain directions are called partial auxetics [6]. Owing to the negative value of this constant, these materials are endowed with very particular characteristics and peculiar mechanical behavior [7]. Some examples are their superior resistance to indentation, shear and fracture, enhanced acoustic absorption, synclastic behavior, variable permeability, and shape memory characteristics [1]. Some geometric models have been developed to justify this unusual behavior; among them, the most common are the reentrant, chiral, and semirigid rotating models (e.g., Ref. [7]). It is commonly accepted that these models always demonstrate auxetic behavior; however, this may not always be true [8]. This study analyzes whether the presence of protruding ribs in a reentrant structure is enough to produce auxetic behavior in reentrant structures. The experimental study of such models, by considering how they are made and conducting experiments on them, is an elaborate and complex task. It is convenient to resort to finiteelement (FE) analysis to analyze them (e.g., Refs. [3,9]). The use of such techniques is a very efficient and a quick way to manipulate and determine the behavior of different reentrant models [10]. Consequently, these routines make it possible to determine the parameters that influence the auxetic behavior of these structures.
2 296 V. H. Carneiro et al. Fig. 1 a Individual cell in reentrant lattice. b Base analyzed reentrant structure The objective of the present article is the study of the parameters that influence the auxetic behavior of reentrant structures using FE analysis, considering the variation in the geometrical and base material characteristics. This study may lead to the tailoring of these structures and permit the application of lattices (periodic structures composed by struts [11]) with a projected PR in practical applications. Additionally, the relative densities of the simulated reentrant structures will be determined considering different geometries so as to generate values of critical relative density in the transition between auxetic and nonauxetic behavior. 2 Methodology The fundamental objective of this study is the definition of the variables that determine the presence of auxetic behavior in a reentrant twodimensional structure (Fig. 1a). To this end, numerical simulations (using FE analysis) were conducted to model a base reentrant structure (Fig. 1b), varying some structural characteristics and applying a quasistatic tensile load (F1 ) on the XXaxis (the value of the load assured that the structures never experienced plastic deformation). This method was adopted so the inertial terms would be negligible. The resultant deformations made it possible to determine the PR of the structure and, consequently, the presence/absence of auxetic behavior. 2.1 Structural characteristics: geometry and base material properties The modified characteristics were divided into two main categories: the geometrical and the base material parameters. In the first category, the variation consisted in changing the length (a), width (c), and initial angle (β) of the ribs of the initial reentrant structures (Fig. 1, Table 1). The base material of the structure was defined as linear elastic and isotropic. This implies that its elastic behavior can be defined by only two of the four basic isotropic elastic Table 1 Initial structural and modified structural characteristics Parameter Initial E (Young s modulus: base material) 200 ν (Poisson s ratio: base material) 0.3 a (Length) 40 c (Width) 6 β (Angle) 45 F (Load) 20 Modified Units GPa mm mm ( ) N constants [12]. In this approach, the selected elastic constants were the Young s modulus and the PR. These constants completely characterize the elastic behavior of the structures. Given that the reentrant structures are represented in two dimensions, they were simplified in the simulations using plane stress conditions. The other elastic constants, the bulk (K ) and shear (G) moduli, can be determined considering the adopted simplification by Eqs. (1) and (2) [13]: E, 2(1 ν) E G=. 2(1 + ν) K = (1) (2) 2.2 Structure simulation: finiteelement analysis characteristics To determine the PR of the structures, whose parameters were varied, a simulation was conducted using FE analysis. The type of simulation used was a linear elastic plane stress model, considering that the base material is isotropic. Thus, the deformation behavior of the body was regulated by Hooke s law (Eq. (3)): σi j = D εi j. (3) The stress (σ ) in the structure is generated by the quasistatic unitary force (F1 : Fig. 1a), applied on the XXaxis to
3 Analysis of the geometrical dependence of auxetic behavior 297 Table 2 Mesh characteristics Mesh settings Value Finally, the PR of the analyzed structures can be simply determined using Eq. (8): Maximum element size Minimum element size 0. Maximum element growth rate Resolution of curvature Resolution of narrow regions the structure (initially in a free body). In isotropic materials, the twodimensional stiffness matrix D is defined by Eq. (4): 1 ν 0 E D = (1 ν 2 ν 1 0. (4) ) ν This relation implies that there are deformations imposed on the structure. The observed deformation may also be generally expressed on a given axis, in the form of strain, by Eq. (5): ε = 1 2 ( u + u T). (5) Using FE analysis, the previously defined equations may be used to determine the strain of the nodes that compose the mesh in which the analyzed body is subdivided. The numerical computation was performed using COMSOL Multiphysics. The mesh created by that software was built using the preset parameter values in the Extra fine mesh function (see Table 2 for settings). To generate the desired results, the software used the MUltifrontal Massively Parallel sparse direct Solver (MUMPS solver). 2.3 Determination of Poisson s ratio of reentrant structures To determine the PR of each analyzed structure and the presence/absence of auxetic behavior, the strain values were monitored in two nodes (Fig. 1). Node 1 is placed on the axis of the imposed tensile load and will only deform in that direction (XXaxis). Node 2 was placed such that it deforms only along the YYaxis, following the expansion/contraction of the protruding ribs. Thus, by the definition and monitoring of these two nodes, it is possible to determine the longitudinal (XXaxis) and transverse (YYaxis) strains of each analyzed structure using Eqs. (6) and (7): ( ) u ε (xx, Structure) = 2 x, node 1, (6) ( ) v ε (yy, Structure) = 2 y, node 2. (7) ν Structure = ε (xx, Structure) ε (yy, Structure). (8) 3 Results and discussion The role of the rib width was verified (Fig. 2) in the deformation mechanism of a reentrant structure. Its value was varied and numerical simulations were conducted, with the parameters mentioned previously, to calculate the PR of the individual reentrant structure. It can be observed in Fig. 2 that the rib width has a direct influence on the value of the PR of a reentrant structure. As the rib width increases, so does the general value of the PR in a reentrant structure. The increase in the PR with the rib width can be interpreted in the following way. When there is a small rib width, there are significant deformations even for small loads. The structure itself is not very rigid and behaves like a spring, forcing a significant vertical expansion. On the other hand, increasing the rib width will generate a stiffer structure. This change will eventually culminate in the loss of auxetic behavior, as the internal space and, consequently, the protruding ribs tend to be eliminated by the increase in the rib width. The role of the rib length (Fig. 3) was analyzed. Its value was varied and numerical simulations were conducted to determine the resulting structure s PR. Analyzing Fig. 3, it can be observed that the rib length is a key parameter in the determination of the PR of a reentrant structure. It is shown that when the rib length increases, the actual PR of the reentrant structure decreases. This can be justified by the spring behavior of the reentrant struc Fig. 2 Variation of structure s PR by changing the rib width (a = 40 mm, β= 45, E = 200 GPa, ν= 0.3)
4 298 V. H. Carneiro et al. Fig. 3 Variation of structure s PR by changing the rib length (c = 6mm,β= 45, E = 200 GPa, ν= 0.3) Fig. 5 Variation of structure s PR by changing the rib angle (a = 40 mm, c = 6mm, E = 200 GPa, ν= 0.3) Fig. 4 Variation of structure s PR by keeping the rib s AR at 5 (β = 45, E = 200 GPa, ν= 0.3) ture. When the rib length is increased, the general structure stiffness decreases. This fact leads to significant deformations and to the vertical expansion that characterizes auxetic behavior. Observing the previous results in Fig. 3, it can be concluded that the auxetic behavior of a reentrant structure depends on the rib length and width. These values are mainly related to the length and width of the ribs, which will determine the stiffness of the structure. Therefore, simulations were conducted to determine the dependence of the PR of the structure on the aspect ratio (AR) between the length and the width of a structure s ribs (Fig. 4). The value of the rib length was varied, but the proportion of the AR was kept constant at a value of 5. According to Fig. 4, it can be observed that when the AR is kept constant, the PR of the structure remains constant as well. Another analyzed parameter was the initial angle between ribs, as shown in Fig. 5. Numerical simulations were conducted with different values of the initial angles, and the importance of a reentrant structure in the deformation mechanism was verified. Fig. 6 Variation of structure s PR by changing the base material PR and Young s modulus (a = 40 mm, c = 6mm,β= 45 ) Observing Fig. 5, it can be concluded that the PR of a reentrant structure is influenced by the initial angle between ribs. When the angle decreases, there is a similar decrease in the value of the structure s PR. However, for extremely low values of rib angles, the PR increases. A decrease in the rib angle generates a decrease in the free interior structural space. In extreme cases, this space ceases to exist, eliminating the reentrant structure. Proceeding to the base material parameters, the PR and Young s modulus of the base material were analyzed to determine their influence on the deformation behavior of a reentrant structure. Geometrical equivalent base structures were simulated based on Fig. 1b, varying the PR and the Young s modulus of the base material. The results are presented in Fig. 6. It is shown the PR of the reentrant structure remains stable when the PR of the base material is changed. Note that the
5 Analysis of the geometrical dependence of auxetic behavior 299 Table 3 PR of reentrant structure for different ARs and rib angles (E = 200 GPa, ν = 0.3) Fig. 7 Variation of structure s PR using the rib angle for different ARs two do not predominate when describing the deformation mechanism of a reentrant structure. As may be observed, the value of the PR of the reentrant structure remained constant when the Young s modulus of the base material was changed. In this way, it is shown that the PR of a reentrant structure is independent of the value of the Young s modulus of the base material. Having isolated all the fundamental parameters that describe the deformation mechanism of a reentrant structure, we can establish that the auxetic behavior will mainly depend on the interaction of the length, width, and angle of the ribs. Because the PR of a reentrant structure remains constant for the same rib AR, these two parameters can be analyzed using only one ratio. With the facts presented, and carrying out numerical simulations, the obtained information was used to create Table 3. Looking at Table 3, it can be observed that there is a dependence between the auxetic behavior, low values of rib angles, and high values of AR. According to the executed simulations and the resulting data, it was possible to elaborate Fig. 7. Boundaries relating the structure s AR and initial rib angle were established that might predict whether a reentrant structure will demonstrate auxetic behavior and show the specific values of the PR. In terms of relative density, it can be observed in Fig. 8 that the values of AR and initial rib angle generate a parabola shape function. When the values of the initial rib angle are extreme (either high or low), the values of the relative density tend to decrease. However, only low values of AR Fig. 8 Relative density of reentrant structures as a function of rib angle and AR tend to increase this effect. It can also be observed that each AR that demonstrates auxetic behavior has a specific value of the critical relative density where the transition between auxetic/nonauxetic behavior takes place. Considering the aforementioned plots, it is suggested that the value of the critical density is lower in the presence of a low AR. In contrast, for low initial rib angles the value of the critical relative density tends to increase. Given that a low AR implies thinner and longer ribs, the overall relative density tends to decrease. However, in the case of the initial rib angle, the structure tends to fold on itself, closing the opening in its interior and generating higher relative density values. 4 Conclusions Considering the results of the executed numerical simulations, it was shown that a reentrant structure, even in the presence of protruding ribs, may not always demonstrate auxetic behavior. This study isolated the length, width (mainly the AR), and initial angle of the structure s ribs
6 300 V. H. Carneiro et al. as the predominant factors that determine auxetic behavior. It was also observed that the characteristics of the base material that composes the structures, such as the constants that describe elastic deformation, may have less influence on the auxetic behavior of a reentrant structure. Limits to the values of length, width, and angles of the ribs were defined to obtain and tailor a predetermined value of the PR of these structures. This allows for the development of structures with a defined PR, even in the project phase, using the same base geometry. According to this formulation, the obtained value of PR is directly related to the unitary reentrant structure. In the case of their application in a lattice, the obtained value of the macroscopic PR may vary slightly, given that the ribs that connect the individual reentrant structures are also elastic. However, as the present study suggests, the main deformation mechanism used to induce auxetic behavior is the bending of the protruding ribs, and this implies a low AR of the ribs. The elastic deformation of the ribs that connect each individual reentrant structure (the ones that do not protrude) is mainly the result of tensile and compressive forces. This last forces, in connection with macroscopic deformation, are negligible compared to the overall reentrant structure expansion. Additionally, the value of the critical relative density at which the transition between auxetic and nonauxetic behavior occurs was determined. It was shown that this value tends to increase for lower initial rib angles. However, in the presence of a low AR, the value of the critical relative densities tends also to decrease. The generated values of the relative density may also be used in a project phase as an input on weight and overall structural performance when projecting an auxetic lattice. References 1. Carneiro, V.H., Puga, H., Meireles, J.: Auxetic materials a review. Mater. Sci. Pol. 31, (2013) 2. Mott, P.H., Roland, C.M.: Limits to Poisson s ratio in isotropic materials general results for arbitrary deformation. Phys. Scr. 87, (2013) 3. Strek, T., Maruszewski, B., Narijczyk, J.W., et al.: Finite element analysis of plate deformation. J. Noncryst. Solids 354, (2008) 4. Norris, A.N.: Extreme values of Poisson s ratio and other engineering moduli in anisotropic materials. J. Mech. Mater. Struct. 1, (2006) 5. Dirrenberger, J., Forest, S., Jeulin, D.: Elastoplasticity of auxetic materials. Comput. Mater. Sci. 64, (2012) 6. Brańka, A.C., Heyes, D.M.: Maćkowiak, Sz, et al.:cubic materials in different auxetic regions linking microscopic to macroscopic formulations. Phys. Status Solidi B 249, (2012) 7. Critchley, R., Corni, I., Wharton, J.A., et al.: A review of the manufacture, mechanical properties and potential applications of auxetic foams. Phys. Status Solidi B 250, (2013) 8. Liu, Y., Hu, H.: A review in auxetic structures and polymeric materials. Sci. Res. Essays 5, (2010) 9. Bückmann, T., Schittny, R., Thiel, M., et al.: On threedimensional dilational elastic metamaterials. N. J. Phys. 16, (2014) 10. Pozniak, A.A., Smardzewski, J., Wojciechowski, K.W.: Computer simulations of auxetic foams in twodimensions. Smart Mater. Struct. 22, (2013) 11. Fan, H.L., Zeng, T., Fang, D.N., et al.: Mechanics of advanced fiber reinforced lattice composites. Acta Mech. Sin. 26, (2010) 12. Du, D.X., Zheng, Q.S., Gao, Y.X.: Consistency between independence theorems and generalized selfconsistent method. Acta Mech. Sin. 13, (1997) 13. Jasiuk, I., Chen, J., Thorpe, M.F.: Elastic moduli of two dimensional materials with polygonal and elliptical holes. Appl. Mech. Rev. 47, (1994)
Poisson s ratio of rectangular antichiral lattices with disorder
Poisson s ratio of rectangular antichiral lattices with disorder Artur A. Poźniak 1 Krzysztof W. Wojciechowski 2 1 Institute of Physics, Poznań Universty of Technology, ul. Nieszawska 13A, 60695 Poznań,
More informationPlanar auxeticity from various inclusions
Planar auxeticity from various inclusions Artur A. Poźniak 1 Krzysztof W. Wojciechowski 2 Joseph N. Grima 3 Luke Mizzi 4 1 Institute of Physics, Poznań Universty of Technology, Piotrowo 3, 6695 Poznań
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More information548 Advances of Computational Mechanics in Australia
Applied Mechanics and Materials Online: 20160725 ISSN: 16627482, Vol. 846, pp 547552 doi:10.4028/www.scientific.net/amm.846.547 2016 Trans Tech Publications, Switzerland Geometric bounds for bucklinginduced
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationComputer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature
Computer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature JAKUB NAROJCZYK KRZYSZTOF W. WOJCIECHOWSKI Institute of Molecular Physics Polish Academy of Sciences ul. M. Smoluchowskiego
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationComputational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure
Vibrations in Physical Systems Vol. 27 (2016) Abstract Computational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure Eligiusz IDCZAK Institute of Applied Mechanics, Poznan University
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationApplication of nanoindentation technique to extract properties of thin films through experimental and numerical analysis
Materials SciencePoland, Vol. 28, No. 3, 2010 Application of nanoindentation technique to extract properties of thin films through experimental and numerical analysis A. WYMYSŁOWSKI 1*, Ł. DOWHAŃ 1, O.
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationMODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD
MODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD Andrzej Skrzat, Rzeszow University of Technology, Powst. Warszawy 8, Rzeszow, Poland Abstract: Userdefined material models which can be used
More informationStress in FlipChip Solder Bumps due to Package Warpage  Matt Pharr
Stress in FlipChip Bumps due to Package Warpage  Matt Pharr Introduction As the size of microelectronic devices continues to decrease, interconnects in the devices are scaling down correspondingly.
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationContent. Department of Mathematics University of Oslo
Chapter: 1 MEK4560 The Finite Element Method in Solid Mechanics II (January 25, 2008) (Epost:torgeiru@math.uio.no) Page 1 of 14 Content 1 Introduction to MEK4560 3 1.1 Minimum Potential energy..............................
More informationNonlocal material properties of single walled carbon nanotubes
Nonlocal material properties of single walled carbon nanotubes J. V. Araújo dos Santos * and C. M. Mota Soares IDMEC, Instituto Superior Técnico, Universidade Técnica de Lisboa, Portugal Av. Rovisco Pais,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationAuxetic Materials A Review
Materials SciencePoland, 31(4), 2013, pp. 561571 http://www.materialsscience.pwr.wroc.pl/ DOI: 10.2478/s1353601301406 Auxetic Materials A Review V. H. CARNEIRO, J. MEIRELES, H. PUGA Department of
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationSEISMIC BASE ISOLATION
SEISMIC BASE ISOLATION DESIGN OF BASE ISOLATION SYSTEMS IN BUILDINGS FILIPE RIBEIRO DE FIGUEIREDO SUMMARY The current paper aims to present the results of a study for the comparison of different base isolation
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationMathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling
Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,
More informationX has a higher value of the Young modulus. Y has a lower maximum tensile stress than X
Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which
More informationLoad Cell Design Using COMSOL Multiphysics
Load Cell Design Using COMSOL Multiphysics Andrei Marchidan, Tarah N. Sullivan and Joseph L. Palladino Department of Engineering, Trinity College, Hartford, CT 06106, USA joseph.palladino@trincoll.edu
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationElastic plastic bending of stepped annular plates
Applications of Mathematics and Computer Engineering Elastic plastic bending of stepped annular plates JAAN LELLEP University of Tartu Institute of Mathematics J. Liivi Street, 549 Tartu ESTONIA jaan.lellep@ut.ee
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationControlling elastic wave with isotropic transformation materials
Controlling elastic wave with isotropic transformation materials Zheng Chang, Jin Hu, a, Gengkai Hu, b, Ran Tao and Yue Wang School of Aerospace Engineering, Beijing Institute of Technology, 0008,Beijing,
More informationGLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE
GLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE Alessandro Spadoni, Massimo Ruzzene School of Aerospace Engineering Georgia Institute of Technology Atlanta, GA 30332 Fabrizio Scarpa
More informationLecture 8 Viscoelasticity and Deformation
HW#5 Due 2/13 (Friday) Lab #1 Due 2/18 (Next Wednesday) For Friday Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, μ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationFabrication and Testing of 2Dimensional ZExpandable Auxetic Textile. Structures for Impact Protective Clothing Applications
2D ZEXPANDABLE AUXETIC TEXTILES FOR IMPACT PROTECTION 1 Fabrication and Testing of 2Dimensional ZExpandable Auxetic Textile Structures for Impact Protective Clothing Applications ASTM Student Project
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationMarch 24, Chapter 4. Deflection and Stiffness. Dr. Mohammad Suliman Abuhaiba, PE
Chapter 4 Deflection and Stiffness 1 2 Chapter Outline Spring Rates Tension, Compression, and Torsion Deflection Due to Bending Beam Deflection Methods Beam Deflections by Superposition Strain Energy Castigliano
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationThis article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and
This article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and education use, including for instruction at the authors institution
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationDesign of inplane piezoelectric sensors for static response by simultaneously optimizing the host structure and the electrode profile
10 th World Congress on Structural and Multidisciplinary Optimization May 1924, 2013, Orlando, Florida, USA Design of inplane piezoelectric sensors for static response by simultaneously optimizing the
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationDESIGN OF AUXETIC SANDWICH PANELS FOR STRUCTURAL APPLICATIONS. Abstract
DESIGN OF AUXETIC SANDWICH PANELS FOR STRUCTURAL APPLICATIONS Li Yang 1, Ola Harrysson, Denis Cormier 3, Harvey West, Chun Park, Kara Peters 1 University of Louisville, Louisville, KY North Carolina State
More informationTHE EFFECT OF GEOMETRY ON FATIGUE LIFE FOR BELLOWS
Advanced Materials Development and Performance (AMDP2011) International Journal of Modern Physics: Conference Series Vol. 6 (2012) 343348 World Scientific Publishing Company DOI: 10.1142/S2010194512003418
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationStatic Equilibrium; Elasticity & Fracture
Static Equilibrium; Elasticity & Fracture The Conditions for Equilibrium Statics is concerned with the calculation of the forces acting on and within structures that are in equilibrium. An object with
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationTolerance Ring Improvement for Reducing Metal Scratch
International Journal of Scientific and Research Publications, Volume 2, Issue 11, November 2012 1 Tolerance Ring Improvement for Reducing Metal Scratch Pattaraweerin Woraratsoontorn*, Pitikhate Sooraksa**
More informationModule 6. Approximate Methods for Indeterminate Structural Analysis. Version 2 CE IIT, Kharagpur
Module 6 Approximate Methods for Indeterminate Structural Analysis Lesson 35 Indeterminate Trusses and Industrial rames Instructional Objectives: After reading this chapter the student will be able to
More information